General Guide to Machining Nickel-Iron Alloys
The Nickel-Iron Alloy Family generally includes INVAR, KOVAR®, Alloys 42, 46, 48, and 52, Alloy 42-6 and magnetic shielding alloys such as MuMetal.
This group of alloys is not hardenable by heat treatment. They can be made harder through cold working only. The annealed hardness for these alloys is generally in the range of RB 70/80, whereas the 1¦4 H to 1¦2 H range for this group of metals, can run between RB 80/96. Material in the annealed condition will be more difficult to machine because it is soft and gummy. The tools tend to plow the metal instead of cutting into it, and do not easily form chips. Surface scale oxide is tightly adherent and penetrates the surface to a greater extent than stainless steels. Machining is considerably improved by descaling the material. If there were standard machinability ratings applied for this series of alloys, Alloy AISI-B-1112 being measured as 100%, the following percentages could be suggested for these chemistries:
INVAR FM -- 60%
KOVAR (ASTM-F15) -- 40%
Alloy 48 -- 40%
It is important to control heat buildup, the major cause of warpage. Suggested coolants are Keycool 2000 or Prime Cut. Whatever lubricant is used for machining, it should not contain sulphur. Sulphur can effect the performance of many sealed electronic parts.
T-15 Alloy, such as Vasco Supreme - manufactured by Vanadium Alloys Company, M-3 Type 2 such as Van Cut Type 2 - manufactured by Vanadium Alloys Company. Congo-manufactured by Braeburn.
For machining with carbide tools, a K-6 manufactured by Kennemetal, Firthite HA manufactured by Firth Sterling, or #370 Carboloy could be used, or a K2S manufactured by Kennemetal, or a Firthite T-04 manufactured by Firth Sterling would be satisfactory. One thing of prime importance is that all feathered or wire edges should be removed from the tools. They should be kept in excellent condition by repeated inspection.
|End cutting edge angle||-||Approximately 7°|
|Nose Radius||-||Approximately .005"|
|Side cutting edge angle||-||Approximately 15°|
|Back rake||-||Approximately 8°|
|Side rake||-||Approximately 8°|
When cutting off, high speed tools are better than carbide tools, and a feed of approximately .001" per revolution should be used. The cutting tools should have a front clearance of about 7° and a fairly big tip - larger than 25° would be helpful.
When drilling a 3/16" diameter hole, a speed of about 40/FPM could possibly be used, and the feed should be about .002" to a .0025" per revolution, for a 1/2" hole, approximately the same speed could be used with a feed of about .0040" to .005" per revolution. The drills should be as short as possible, and it is desirable to make a thin web at the point by conventional methods. By conventional methods, we mean do not notch or make a crank shaft grind. It is suggested that heavy web type drills with nitrided or electrolyzed surfaces be used. The hole, of course, should be cleaned frequently in order to remove the chips, which will gall, and also for cooling. The drill should be ground to an included point angle of 118° to 120°.
Reaming speeds should be half the drill speed, but the feed should be about three times the drill speed. It is suggested that the margin on the land should be about .005" to .010", and that the chamfer should be .005" to .010" and the chamfer angle about 30°. The tools should be as short as possible, and have a slight face rake of about 5° to 8°.
Controlled Expansion AlloysEd Fagan Europe Ltd. stocks a variety of similar alloys for low expansion, controlled expansion, glass-to-metal or ceramic sealing applications that may also satisfy your needs. EFI carries:
And we also have a large selection of other types of specialty metals and alloys for high technology applications, including:
Soft Magnetic Alloys
Refractory Metals and Alloys
Hard to Find Materials